1

Hyperbolic Metamaterials

Igor I. Smolyaninov Department of Electrical and Computer Engineering, University of Maryland, College Park, MD 20742, USA

Hyperbolic metamaterials were originally introduced to overcome the diffraction limit of optical imaging.

Soon thereafter it was realized that hyperbolic

metamaterials demonstrate a number of novel phenomena resulting from the broadband singular behavior of their density of photonic states. These novel phenomena and applications include super resolution imaging, new stealth technologies,

enhanced

hyperconductivity,

quantum-electrodynamic

superconductivity,

and

interesting

effects,

thermal

gravitation

theory

analogues. Here we briefly review typical material systems, which exhibit hyperbolic

behavior

metamaterials.

and

outline

important

applications

of

hyperbolic

2

Table of Content 1. Hyperbolic metamaterial geometries and basic properties

3

2. Super-resolution imaging using hyperbolic metamaterials: the hyperlens

8

3. Consequences of singular photonic density of states: radiative decay engineering, thermal hyper-conductivity, and new stealth technologies

13

4. Photonic hypercrystals

18

5. Superconducting hyperbolic metamaterials

26

6. Gravitation theory analogs based on hyperbolic metamaterials

31

7. Summary

38

8. References

39

3

1. Hyperbolic metamaterial geometries and basic properties Hyperbolic metamaterials are extremely anisotropic uniaxial materials, which behave like a metal in one direction and like a dielectric in the orthogonal direction. Originally introduced to overcome the diffraction limit of optical imaging [1-2], hyperbolic metamaterials demonstrate a number of novel phenomena resulting from the broadband singular behavior of their density of photonic states [3], which range from super resolution imaging [2,4,5] to enhanced quantum-electrodynamic effects [6,7,8], new stealth technology [9], thermal hyperconductivity [10], high Tc superconductivity [11,12], and interesting gravitation theory analogues [3, 13-17]. In the early days of metamaterial research it was believed that only artificially structured materials may exhibit hyperbolic properties. However, later on it was realized that quite a few natural materials may exhibit hyperbolic properties in some frequency ranges [11,18]. Moreover, even the physical vacuum may exhibit hyperbolic metamaterial properties if subjected to a very strong magnetic field [19]. Basic electromagnetic properties of hyperbolic metamaterials may be understood by considering a non-magnetic uniaxial anisotropic material with dielectric permittivities x=y=1 and z=2. Any electromagnetic field propagating in this material may be expressed as a sum of ordinary and extraordinary contributions, each of these being a sum of an arbitrary number of plane waves polarized in the ordinary (Ez=0) and extraordinary (Ez≠0) directions. Let us define a “scalar” extraordinary wave function as Ez so that the ordinary portion of the electromagnetic field does not contribute to . Maxwell equations in the frequency domain results in the following wave equation for if 1 and 2 are kept constant inside the metamaterial [3]:

2 1 2 2 c2 1z 2 2 x 2 y 2

2

(1.1)

4

While in ordinary elliptic anisotropic media both 1 and 2 are positive, in hyperbolic metamaterials 1 and 2 have opposite signs. These metamaterials are typically composed of multilayer metal-dielectric or metal wire array structures, as shown in Fig. 1. The opposite signs of 1 and 2

lead to two important consequences. For

extraordinary waves in a usual uniaxial dielectric metamaterial, the dispersion law

k xy2

2

k z2

1

2 c2

(1.2)

describes an ellipsoid in the wave momentum (k-) space (which reduces to a sphere if

1 2 , as shown in Fig.2(a)). The absolute value of the k-vector in such a material is finite which leads to the usual diffraction limit on resolution of regular optics. The phase space volume enclosed between two such equi-frequency surfaces is also finite, corresponding to a finite density of photonic states. However, when one of the components of the dielectric permittivity tensor is negative, eq.(1.2) describes a hyperboloid in the phase space (Fig. 2(b)). As a result, the absolute value of the k-vector is not limited, thus enabling super-resolution imaging with hyperbolic metamaterials. Moreover, the phase space volume between two such hyperbolloids (corresponding to different values of frequency) is infinite (see Fig. 2(c)). The latter divergence leads to an infinite density of photonic states. While there are many mechanisms leading to a singularity in the density of photonic states, this one is unique as it leads to the infinite value of the density of states for every frequency where different components of the dielectric permittivity have opposite signs. It is this behavior which lies in the heart of the robust performance of hyperbolic metamaterials: while disorder can change the magnitude of the dielectric permittivity components, leading to a deformation of the corresponding hyperboloid in the phase (momentum) space, it will remain a hyperboloid

5

and will therefore still support an infinite density of states. Such effective medium description will eventually fail at the point when the wavelength of the propagating mode becomes comparable to the size of the hyperbolic metamaterial unit cell a, introducing a natural wave number cut-off:

k max 1 / a

(1.3)

Depending on the metamaterial design and the fabrication method used, the unit cell size in optical metamaterials runs from a~10 nm (in semiconductor [20] and metaldielectric layered structures [6]) to a~100 nm (in nanowire composites [21],[22]). Since the “hyperbolic" ehnancement factor in the density of states [3] scales as

k ( ) 0 ( ) max /c

3

(1.4)

where 0~2 is the free-space result, even with the cut-off taken into account, the hyperbolic singularity leads to the optical density of states enhancement by a factor of 103-105. Physically, the enhanced photonic density of states in the hyperbolic metamaterials originates from the waves with high wave numbers that are supported by the system. Such propagating modes that can achieve X-ray wavelengths at optical frequencies, do not have an equivalent in ”regular" dielectrics where k / c . Since each of these waves can be thermally excited, a hyperbolic metamaterial shows a dramatic enhancement in the radiative transfer rates. As has been mentioned above, artificial hyperbolic metamaterials are typically composed of multilayer metal-dielectric or metal wire array structures, as shown in Fig. 1. For the multilayer geometry the diagonal components of the metamaterial permittivity can be calculated based on the Maxwell-Garnett approximation as follows:

6

1 xy n m 1 n d ,

2 z

m d 1 n m n d

(1.5)

where nis the volume fraction of the metallic phase, and m0 are the dielectric permittivities of the metal and dielectric, respectively [23]. The validity of Maxwell-Garnett approximation has been clearly demonstrated in ref.[23]. Analytical calculations based on the Maxwell-Garnett approximation performed for periodic array of metal nanolayers were confronted with exact numerical solutions of Maxwell equations. Excellent agreement between numerical simulations and analytical results was demonstrated. The Maxwell-Garnett approximation may also be used for a wire array metamaterial structure [23]. In this case the diagonal components of the permittivity tensor may be obtained as

1 x, y

2n m d (1 n) d ( d m ) , 1 n( d m ) 2n d

2 z n m 1 n d

(1.6)

Since both m and d depend on frequency, the frequency regions where 1 and 2 have opposite signs may be typically found for both multilayer and wire array geometries. Depending on the actual signs of 1 and 2, the phase space shape of the hyperbolic dispersion law may be either a one-sheet (2>0 and 1

Hyperbolic Metamaterials

Igor I. Smolyaninov Department of Electrical and Computer Engineering, University of Maryland, College Park, MD 20742, USA

Hyperbolic metamaterials were originally introduced to overcome the diffraction limit of optical imaging.

Soon thereafter it was realized that hyperbolic

metamaterials demonstrate a number of novel phenomena resulting from the broadband singular behavior of their density of photonic states. These novel phenomena and applications include super resolution imaging, new stealth technologies,

enhanced

hyperconductivity,

quantum-electrodynamic

superconductivity,

and

interesting

effects,

thermal

gravitation

theory

analogues. Here we briefly review typical material systems, which exhibit hyperbolic

behavior

metamaterials.

and

outline

important

applications

of

hyperbolic

2

Table of Content 1. Hyperbolic metamaterial geometries and basic properties

3

2. Super-resolution imaging using hyperbolic metamaterials: the hyperlens

8

3. Consequences of singular photonic density of states: radiative decay engineering, thermal hyper-conductivity, and new stealth technologies

13

4. Photonic hypercrystals

18

5. Superconducting hyperbolic metamaterials

26

6. Gravitation theory analogs based on hyperbolic metamaterials

31

7. Summary

38

8. References

39

3

1. Hyperbolic metamaterial geometries and basic properties Hyperbolic metamaterials are extremely anisotropic uniaxial materials, which behave like a metal in one direction and like a dielectric in the orthogonal direction. Originally introduced to overcome the diffraction limit of optical imaging [1-2], hyperbolic metamaterials demonstrate a number of novel phenomena resulting from the broadband singular behavior of their density of photonic states [3], which range from super resolution imaging [2,4,5] to enhanced quantum-electrodynamic effects [6,7,8], new stealth technology [9], thermal hyperconductivity [10], high Tc superconductivity [11,12], and interesting gravitation theory analogues [3, 13-17]. In the early days of metamaterial research it was believed that only artificially structured materials may exhibit hyperbolic properties. However, later on it was realized that quite a few natural materials may exhibit hyperbolic properties in some frequency ranges [11,18]. Moreover, even the physical vacuum may exhibit hyperbolic metamaterial properties if subjected to a very strong magnetic field [19]. Basic electromagnetic properties of hyperbolic metamaterials may be understood by considering a non-magnetic uniaxial anisotropic material with dielectric permittivities x=y=1 and z=2. Any electromagnetic field propagating in this material may be expressed as a sum of ordinary and extraordinary contributions, each of these being a sum of an arbitrary number of plane waves polarized in the ordinary (Ez=0) and extraordinary (Ez≠0) directions. Let us define a “scalar” extraordinary wave function as Ez so that the ordinary portion of the electromagnetic field does not contribute to . Maxwell equations in the frequency domain results in the following wave equation for if 1 and 2 are kept constant inside the metamaterial [3]:

2 1 2 2 c2 1z 2 2 x 2 y 2

2

(1.1)

4

While in ordinary elliptic anisotropic media both 1 and 2 are positive, in hyperbolic metamaterials 1 and 2 have opposite signs. These metamaterials are typically composed of multilayer metal-dielectric or metal wire array structures, as shown in Fig. 1. The opposite signs of 1 and 2

lead to two important consequences. For

extraordinary waves in a usual uniaxial dielectric metamaterial, the dispersion law

k xy2

2

k z2

1

2 c2

(1.2)

describes an ellipsoid in the wave momentum (k-) space (which reduces to a sphere if

1 2 , as shown in Fig.2(a)). The absolute value of the k-vector in such a material is finite which leads to the usual diffraction limit on resolution of regular optics. The phase space volume enclosed between two such equi-frequency surfaces is also finite, corresponding to a finite density of photonic states. However, when one of the components of the dielectric permittivity tensor is negative, eq.(1.2) describes a hyperboloid in the phase space (Fig. 2(b)). As a result, the absolute value of the k-vector is not limited, thus enabling super-resolution imaging with hyperbolic metamaterials. Moreover, the phase space volume between two such hyperbolloids (corresponding to different values of frequency) is infinite (see Fig. 2(c)). The latter divergence leads to an infinite density of photonic states. While there are many mechanisms leading to a singularity in the density of photonic states, this one is unique as it leads to the infinite value of the density of states for every frequency where different components of the dielectric permittivity have opposite signs. It is this behavior which lies in the heart of the robust performance of hyperbolic metamaterials: while disorder can change the magnitude of the dielectric permittivity components, leading to a deformation of the corresponding hyperboloid in the phase (momentum) space, it will remain a hyperboloid

5

and will therefore still support an infinite density of states. Such effective medium description will eventually fail at the point when the wavelength of the propagating mode becomes comparable to the size of the hyperbolic metamaterial unit cell a, introducing a natural wave number cut-off:

k max 1 / a

(1.3)

Depending on the metamaterial design and the fabrication method used, the unit cell size in optical metamaterials runs from a~10 nm (in semiconductor [20] and metaldielectric layered structures [6]) to a~100 nm (in nanowire composites [21],[22]). Since the “hyperbolic" ehnancement factor in the density of states [3] scales as

k ( ) 0 ( ) max /c

3

(1.4)

where 0~2 is the free-space result, even with the cut-off taken into account, the hyperbolic singularity leads to the optical density of states enhancement by a factor of 103-105. Physically, the enhanced photonic density of states in the hyperbolic metamaterials originates from the waves with high wave numbers that are supported by the system. Such propagating modes that can achieve X-ray wavelengths at optical frequencies, do not have an equivalent in ”regular" dielectrics where k / c . Since each of these waves can be thermally excited, a hyperbolic metamaterial shows a dramatic enhancement in the radiative transfer rates. As has been mentioned above, artificial hyperbolic metamaterials are typically composed of multilayer metal-dielectric or metal wire array structures, as shown in Fig. 1. For the multilayer geometry the diagonal components of the metamaterial permittivity can be calculated based on the Maxwell-Garnett approximation as follows:

6

1 xy n m 1 n d ,

2 z

m d 1 n m n d

(1.5)

where nis the volume fraction of the metallic phase, and m0 are the dielectric permittivities of the metal and dielectric, respectively [23]. The validity of Maxwell-Garnett approximation has been clearly demonstrated in ref.[23]. Analytical calculations based on the Maxwell-Garnett approximation performed for periodic array of metal nanolayers were confronted with exact numerical solutions of Maxwell equations. Excellent agreement between numerical simulations and analytical results was demonstrated. The Maxwell-Garnett approximation may also be used for a wire array metamaterial structure [23]. In this case the diagonal components of the permittivity tensor may be obtained as

1 x, y

2n m d (1 n) d ( d m ) , 1 n( d m ) 2n d

2 z n m 1 n d

(1.6)

Since both m and d depend on frequency, the frequency regions where 1 and 2 have opposite signs may be typically found for both multilayer and wire array geometries. Depending on the actual signs of 1 and 2, the phase space shape of the hyperbolic dispersion law may be either a one-sheet (2>0 and 1